# this file is part of refractiveindex.info database
# refractiveindex.info database is in the public domain
# copyright and related rights waived via CC0 1.0

REFERENCES: "<a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.agf\">OHARA Zemax catalog 2017-11-30</a> (obtained from <a href=\"http://www.ohara-inc.co.jp/en/product/optical/list/\">http://www.ohara-inc.co.jp</a>)<br>See also <a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.pdf\">OHARA glass data sheets</a>"
COMMENTS: ""
DATA:
  - type: formula 3 
    range: 0.3 2.4
    coefficients: 3.2498918 -0.010466366 2 0.048000686 -2 0.0031859922 -4 -0.00015447369 -6 2.6258671e-05 -8
  - type: tabulated k
    data: |
        0.360 1.3193E-05
        0.370 4.8898E-06
        0.380 2.3482E-06
        0.390 1.3369E-06
        0.400 7.9088E-07
        0.420 3.1889E-07
        0.440 1.5024E-07
        0.460 7.7690E-08
        0.480 4.2250E-08
        0.500 2.3945E-08
        0.550 8.7623E-09
        0.600 9.5589E-09
        0.650 1.0355E-08
        0.700 5.5732E-09
SPECS:
    n_is_absolute: false
    λ_is_vacuum: false
    temperature: 25.0 °C
    coefficients_of_thermal_dispersion: 1.722e-05 0.0 0.0 0.0 0.0 0.0
    n_d: 1.846658
    V_d: 23.885544
    glass_code: 847239
    glass_status: preferred
    density: 5.53 g/cm<sup>3</sup>
    coefficient_of_thermal_expansion_1: 7.8e-06 K<sup>-1</sup>
    coefficient_of_thermal_expansion_2: 8.7e-06 K<sup>-1</sup>
    ΔP_gF: 0.0134
    acid_resistance: 52.2
    phosphate_resistance: 3.2
